International Journal of Engineering Science Invention ISSN (Online): 2319 – 6734, ISSN (Print): 2319 – 6726 www.ijesi.org Volume 3 Issue 5ǁ May 2014 ǁ PP.67-72

Dry Sliding Wear Behavior Of Carburized 20mncr5 Alloy Steel Sandeep S Kadam1, Prof. S. D. Ambekar2 1,

Research Scholar Post graduate Student, Mechanical Engineering Department, 2, Asst. Professor, Mechanical Engineering Department Department of Mechanical Engineering, Government College of Engineering Aurangabad Dr. Babasaheb Ambedkar University Aurangabad, India

ABSTRACT: This research is limited to study the wear resistance of carburized 20MnCr5 (SAE 5120) alloy steel, which has wide application in industries like gears, shafts, bearings, pins etc. The abrasive wear study is performed on pin-on-disc tribotester. Sliding velocity of 0.8 m/s, 1.6 m/s, 2.4 m/s, Sliding Distance of 1200 m, 1400 m, 1600 m and Load of 3 kg, 4 kg and 5 kg were used to evaluate the wear resistance.

KEYWORD: Carburizing, Abrasive wear I.

INTRODUCTION

The equation that relates the wear rate with the applied load was at first established by Holm in 1940. This citation can be found in Archard’s paper, which is considered as the main reference for the modeling of wear rate in sliding systems. Holm assumed the wear as an atomic process. The wear rate (worn volume per unit sliding distance) W isgiven by

Where Z is the number of atoms removed per atomicencounter, F is the applied load, and is the flow pressure of worn surface. Furthermore, the term Z can only be interpreted as a probability of atomic removal. 1 This modeling depends on the kind of deformationassumed for the asperities, which Holm considered theplastic deformation as predominant for the materialremoval. To this problem, Archard demonstrated that tosatisfy a linear relationship between the wear rate and theapplied load, some hypothesis on the shape of debrisshould be made, which implies in a new comprehension onthe effective mechanism of material removal.Greenwood and Williansomadded to the Archardtheory, the nature of deformation, considering the heightsof asperities in contact. Their work and many others applied a probabilistic approach for the roughness of Surfaces in contact. However, there are few models withthis approach for the wear coefficient.

II. The plastic contact area

ARCHARD MODEL AS AN INITIAL VALUE PROBLEM can be defined as,

where F and py were defined in Eq. (1). Following the Archard model the worn volume V is given by,

where k is the wear coefficient and x is the sliding distance. Putting Eq. (2) in Eq. (3) one can obtain,

On the other hand, the worn volume can be defined by the following equation where A is the apparent contact area and h is an averageheight corresponding to the material removal. Theidentities defined in Eqs. (4) and (5) lead to

www.ijesi.org

67 | Page

Dry Sliding Wear Behavior Of Carburized… where p is the average normal stress. Steel has many practical applications in every aspects of life. The steel is being divided as low carbon steel, medium carbon steel, high carbon steel, Low carbon steel has carbon steel has carbon content of 0.15%0.45%. As the carbon content increases, the metal becomes harder and stronger but less ductile and more difficult to weld. 20MnCr5 (SAE 5120) categorized as the low carbon alloy steel grade. Category

Steel

Class

Alloy steel

Type

Standard United States: ASTM A322, ASTM A331 , ASTM A519 , SAE J404 , SAE J770 , UNS G51200 France: AFNOR 20 MC 5

Designations

III.

Germany: DIN 1.7147

CARBURIZED HEAT TREATMENT

Carburizing, a surface treatment applied to a part to ensure beneficial surface compressive stresses and increased hardness, improves wear and fatigue resistance.In many machine parts it is required to have hard case comparative to the core e.g. Shafts, gears etc. so that the core can stand the shocks, impact and hard case can stand wear as with increase in the hardness materials loses its ductility and weld ability and becomes brittle. Carburizing introduces a gradient in the surface microstructure and mechanical properties. The hardness and strength of martensite increase with increasing carbon content. 3.1 Sequence of the Heat treatment done on 20MnCr5 Sequence

Process

Temperature

I

Carburizing

900⁰C, 2 hr

II

Quenching

680 ⁰C, Oil quenched

III

Tempering

160 ⁰C , 1.5 hr

3.2 Chemical analysis after Carburizing Heat treatment Elements

RAW Sample

Carburized Sample

%C % Mn

0.17 1.19

0.201 1.12

% Cr

1

1.1

% Ni

0.1

0.1

% Mo %S

0.02 0.021

0.02 0.023

%P

0.024

0.027

% Si

0.25

0.24

IV.

SPECIMEN AND TRIBOLOGY

Case carburized Specimens of 20Mncr5 are prepared for 25 mm length and 10 mm diameter.Combination of Tribological conditions i.e. load, sliding velocity and sliding distance were analyzed

www.ijesi.org

68 | Page

Dry Sliding Wear Behavior Of Carburizedâ&#x20AC;Ś for studying the wear property of the samples on Pin-On-Disc tribotester.Material Samples were used as a Pin for the experimentation and Alumina used as Counterpart (Disc).Experiment is carried out for the three levels of load, Sliding velocity and Sliding distance Load (kg) Sliding velocity (m/s) Sliding Distance (m)

3 0.8 1200

4 1.6 1400

5 2.4 1600

Taguchi L9 array is selected for carrying out the experimentation and weight loss in grams is measured after every trial.

V.

TAGUCHI L9 ARRAY Table 1

Sliding Velocity

Sliding Distance

3

0.8

1200

Material loss 0.0064333

3

1.6

1400

0.0176663

3

2.4

1600

0.0168667

4

0.8

1400

0.0208667

4

1.6

1600

0.0182327

4

2.4

1200

0.0064333

5

0.8

1600

0.0655530

5

1.6

1200

0.0170000

5

2.4

1400

0.0074611

Table 1 Taguchi L9 Array

VI.

RESULTS

6.1 Main effect Plots Main Effects Plot for mean : Carburizing sample load

sliding velocity

Mean of Avg. Material loss

0.03

0.02

0.01 3

4 sliding distance

5

1200

1400

1600

0.8

1.6

2.4

0.03

0.02

0.01

Frommain effect plot it is observed load and sliding distance has direct effect and sliding velocity has inverse effect on material loss.Behavior of wear with respect to load is in compliment with the findings of Xiaoliang Shieta,Min-Soo Suh eta, H.X. Zhu eta, M. Singh eta.

www.ijesi.org

69 | Page

Dry Sliding Wear Behavior Of Carburizedâ&#x20AC;Ś Behavior of wear with respect to sliding distance is in compliment with the findings of Yasin Alemdageta,Min-Soo Suh eta, J.D. Bressan eta, Temel Savaskan eta.Behavior of wear with respect to sliding velocity is in compliment with the findings of Xiaoliang Shieta 6.2 Interaction Plot Interaction Plot for carburised sample 0.8

1.6

2.4

1200

1400

1600

0.025

0.000 0.050 Sliding Velocity

0.025

Sliding Velocity 0.8 1.6 2.4

0.000

Sliding Distance

Wear is reduced with increase in sliding velocity with decrease in loading condition for different sliding distance conditions.For different load conditions, wear is increased with increase in sliding distance with reduces sliding velocity. Time required for completing a particular wear distance is reduced with increase in sliding velocity. When load is 3 kg and sliding distance is increasing, wear is decreasing. When load is 4 kg and 5kg and increase in sliding distance, wear decreases initially and then increases.Maximum wear is observed when sliding velocity is at minimum and sliding distance is increasing and minimum wear is obtained when sliding velocity is at maximum and sliding distance is increasing. 6.3 ANOVA table Table 2 Source

DF

Seq SS

F

P

2

0.0035246

0.0035246

0.0017623

20.68

0.046

Sliding Velocity

2

0.0012767

0.0012767

0.0006383

7.49

0.118

Sliding Distance

2

0.0053023

0.0053023

0.0026512

31.10

0.031

Error

2

0.0001705

0.0001705

0.0000852

Total

8

0.0102741

Table 2 Anova table S = 0.00923220 R-Sq = 98.34% R-Sq(adj) = 93.36% From table it is observed that the sliding distance is the most effecting parameter followed by load and sliding velocity. 6.4 Regression analysis Therelationship between the control factors Sliding Velocity, load, Sliding distance and the output performance wear are obtained by regression analysis. Wear = - 0.0576 + 0.0101 Load - 0.0171 Sliding Velocity + 0.000045 Sliding Distance

www.ijesi.org

70 | Page

Dry Sliding Wear Behavior Of Carburizedâ&#x20AC;Ś VII.

MICROSTRUCTURE

7.1 Raw Material

7.2 Carburized Sample

Carburized sample shows Low carbon tempered martensite with bainitic structure& 5 % free ferrite is observed in martensitic matrix. Raw material shows normalized ferrite VIII.

CONCLUSION

[1] Carburizedheat treatment improves the microstructure and wear property of the material as amount of free ferrite observed in carburized heat treatment is less as compared to rawmaterial. [2] Carbon percentage is increased after carburizing heat treatment hence carburizing heat treatment is successfully done. [3] Minimum wear of cryogenically treated samples is obtained when load is 4 kg sliding distances 1200 m and sliding velocity is 2.4 m/s.

www.ijesi.org

71 | Page

Dry Sliding Wear Behavior Of Carburized… REFFERENCES [1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12]

Claudio R. Avila da Silva Jr., Giuseppe Pintaude, “Uncertainty analysis on the wear coefficient of Archard model” , Elsevier ,Tribology International 41 (2008) 473–481 J.P. Wise, G. Krauss, D.K. Matlock, “Microstructure and Fatigue Resistance of Carburized Steels”, 20th ASM Heat Treating Society Conference Proceedings, 9-12 October 2000. P. Rangaswamy, C.P. Scherer, M.A.M. Bourke, “Experimental measurements and numerical simulation of stress and microstructure in carburized 5120 steel disks”, Materials Science and Engineering A298 (2001) 158–165, Elsevier. Xiaoliang Shi, Mang Wang , Wenzheng Zhai, Zhiwei Zhu,Zengshi Xu, Qiaoxin Zhang, Siyuan Song, Jie Yao, Abid Qamar ud Din, “ Friction and wear behaviour of NiAl-10wt%Ti3SiC2 composites”, wear 303(2013) 9-20,Elsevier. H.X. Zhu, S.K. Liu, X.J. Bai, Z.J. Li, “Sliding wear behaviour of planar random zinc-alloy matrix composites”, wear 199 (1996) 8288, Elsevier. Min-Soo Suh, Young-Hun Chae, Seock-Sam Kim, “Friction and wear behaviour of structural ceramics sliding against Zirconia”, wear (2008) 800-806, Elsevier. M. Singh, D. P. Mondal, O. P. Modi, A. K. Jha, “Two-body abrasive wear behaviour of aluminium alloy-sillimanite particle reinforced composite”, wear 253 (2002) 357-368, Elsevier. Yasin Alemdag, Temel Savaskan, “Mechanical and tribological properties of Al-40Zn-Cu alloys”, Tribology International 42(2009) 176-182, Elsevier. J.D. Bressan, D. P. Daros, A. Sokolowski, R. A. Mesquita, C.A. Barbosa, “ Influence of hardness on the wear resisitance of 17-4 PH stainless steel evaluated by the pin- on-disc testing”, Journal of material processing technology 205 (2008) 353-359, Elsevier. Temel Savaskan, Osman Bican, Yasin Alemdag, “Developing aluminium-zinc-based a new alloy for tribological application”, J Mater Sci (2009) 44:1969-1976 Temel Savaskan, Osman Bican, “Dry sliding friction and wear properties of Al-25Zn-3Cu-3Si alloy”, Tribology International 43(2010)1346-1352, Science direct. Mechanical Engineering (NCAME-2012)”, World Journal of Science and Technology 2012, 2(4):53-59

www.ijesi.org

72 | Page

K0351067072
K0351067072